Presentation on theme: "Anodic Aluminum Oxide. Introduction Objective: Fabricate ordered arrays of structures on the nanometer scale using porous alumina templates."— Presentation transcript:
Anodic Aluminum Oxide
Introduction Objective: Fabricate ordered arrays of structures on the nanometer scale using porous alumina templates.
Motivation: General What is Anodic Porous Alumina? Aluminum oxide grown on an Al substrate in an electrolytic cell. The resulting structure consists of an array of tunable nanometer-sized pores surrounded by an alumina backbone. Purpose: To understand the mechanisms involved in the growth and ordering of anodic porous alumina. Motivation: Why do we want to fabricate nanostructures? Interest in using anodic porous alumina as a nano- template to fabricate nanometer-sized structures (e.g. nanofabrication of quantum dots). 1. Fundamental physical interest in the nanometer size regime. Properties of nano- sized structures are different from their bulk and molecular counterparts. 2. Technological applications as electronic and optical devices.
Microfiltration. Optical waveguides and photonic crystals for optical circuits. Template for carbon nanotube growth for electronic, mechanical applications. Ordered arrays of quantum dots for lasers, photodetectors. ULSI memory devices and ICs. Porous Alumina used as optical waveguide. H. Masuda, et. al., Jpn. J. Appl. Phys. 38, L1403 (1999). Commercially available Anopore filter. pec_prep/filter2.html Ordered arrays of carbon nanotubes fabricated using a porous alumina template. J. Li, et al., Appl. Phys. Lett. 75(3), 367 (1999). 1. Physics: Explore optical, electrical, and magnetic quantum confinement. 2. Engineering: Motivation: Applications
Overview of Anodic Oxide Films Two main types of anodic oxide films can be grown depending on the nature of the electrolyte: 1. Barrier-Type Films: Grown Oxide Insoluble in Electrolyte Nearly Neutral Electrolytes (pH 5-7) 2. Porous-Type Films: Grown Oxide Slightly Soluble in Electrolyte Aqueous Sulfuric, Oxalic, and Phosphoric Acid Electrolytes Fabrication Anodize aluminum in electrolyte (e.g. Oxalic Acid)
Anodize aluminum in electrolyte (e.g. Oxalic Acid). Oxide grows at the metal/oxide and oxide/electrolyte interfaces, pores initiate at random positions by field-assisted dissolution at the oxide/electrolyte interface. Ordering requires appropriate potentials and long anodization times. Ordering results from repulsion between neighboring pores due to mechanical stress at the metal/oxide interface. Apparatus H. Masuda and K. Fukuda, Science 268, 1466 (1995). Resulting Structure Porous Alumina
V.P. Parkhutik, and V.I. Shershulsky, J. Phys. D:Appl. Phys. 25, 1258 (1992). Oxide growth proceeds via ionic conduction and reaction of Al cations and oxygen containing anions under the influence of an applied field. (e.g. 2Al + + 3OH - Al 2 O 3 +3H + +6e - ) Pores initiate at random positions through field-assisted dissolution of the oxide at the oxide/electrolyte interface. Initially oxide growth dominates. (I) Dissolution becomes competitive, barrier layer thins, and pores initiate. (II) Approaches steady state where both mechanisms occur at roughly the same rate. (III and IV) Overview of Film Anodization
Ordered Oxalic Ordered Nano-Templates Near-Ordered Sulfuric Tunable diameters and spacings from 20 nm to 500 nm. Polycrystalline structure: ordered micron-sized domains, defects at grain boundaries. Low temperature growth produces unordered 4-10 nm arrays.
Ordered Growth of Porous Alumina Ordered pore arrays obtained in three different electrolytes for long anodization times and appropriate voltages (specific for each electrolyte). Polycrystalline structure with perfectly ordered domains a few microns in size. Defects occur at grain boundaries.
H. Masuda et al., Jpn. J. Appl. Phys. 35, L126 (1996). Porous alumina used as an evaporation mask to grow quantum dots. Thermally Evaporated Nano-Dots: Gold
Overview: Mask Processing 7. Remove collodion and place alumina on desired substrate. H. Masuda et al., Jpn. J. Appl. Phys. 35, L126 (1996). AFM of Unopened Barrier Layer (1 m x 1 m) Anodize sample for a long time to achieve ordered pores. 2. Chemically remove the alumina in a mixture of phosphoric and chromic acid. 3. Anodize sample for a short time. 4. Coat top surface of alumina with a polymer (collodion) to protect it from further processing. 5. Remove Al Substrate in a saturated HgCl 2 solution. 6. Remove the barrier layer in 5 wt.% Phosphoric Acid.
Procedure: Anodization Apply black wax around the area that you want to anodize. Electropolish Aluminum surface to make it smooth. Anodize the sample that should be ordered for 15 hours in oxalic acid. Anodize the sample that should be disordered for 1 hour in oxalic acid.
Procedure: Anodization (cont.) Chemically remove the alumina in a mixture of phosphoric and chromic acid. Anodize both samples for one hour in oxalic acid. Coat top surface of alumina with a polymer (collodion) to protect it from further processing.
Procedure: Anodization (cont.) Remove Al substrate in a saturated HgCl 2 solution. Use a piece of silicon to pick up oxide and polymer and move to 5 wt. % phosphoric acid. This removes barrier layer. Remove collodion and place alumina on desired substrate- silicon for SEM characterization and quartz for UV-Vis characterization.
Procedure: Thermal Evaporation Remove AAO with double stick tape. Thermally Evaporate Gold onto all Samples –Must be done one sample at a time, because alignment is critical. –Gold layer should be ~50nm thick.
Results: AFM Characterization- disordered Au dots
Results: AFM Characterization- ordered Au dots
Results: SEM Characterization- silicon substrate Ordered AAO (100k magnification)Unordered AAO (100k magnification) Ordered Au dots (100k magnification) Unordered Au dots (100k magnification)
Results: UV-Vis Characterization- quartz substrate Ordered Array Disordered Array Place drop of magic oil on microscope slide to get rid of Newton’s rings Place sample in spectrophotometer. Scan from 300 to 1200nm.